EFFICIENCY OF INTERACTION OF INTERSTITIAL CARBON WITH OXYGEN, TIN, AND SUBSTITUTION CARBON IN IRRADIATED SILICON


 Ashlyn Dickerson
 3 years ago
 Views:
Transcription
1 M.I. GRITSENKO, O.O. KOBZAR, Yu.V. POMOZOV et al. EFFICIENCY OF INTERACTION OF INTERSTITIAL CARBON WITH OXYGEN, TIN, AND SUBSTITUTION CARBON IN IRRADIATED SILICON M.I. GRITSENKO, 1 O.O. KOBZAR, 1 YU.V. POMOZOV, 2 M.G. SOSNIN, 2 L.I. KHIRUNENKO 2 1 Taras Shevchenko Chernigiv State Pedagogical University (53, Get mana Polubotka Str., Chernigiv, Ukraine; o. a. gmail. com ) PACS uf c Institute of Physics, Nat. Acad. of Sci. of Ukraine (46, Prosp. Nauky, Kyiv 03680, Ukraine) The infrared Fourier spectroscopy technique is used for the investigation of the efficiency of interaction of interstitial carbon with the basic technological impurities in silicon, oxygen and substitution carbon, as well as with an isoelectronic impurity, tin. It is shown that the probabilities of the interaction of interstitial carbon with interstitial oxygen and substitution carbon are close. It is found that interstitial carbon in tindoped Si is less thermostable than that in Si, and the temperature of its complete annealing gradually decreases with increasing the tin concentration. It is shown that the probability of the interaction of interstitial carbon with tin exceeds the probability of its interaction with oxygen and onsite carbon by a factor of Introduction Carbon in silicon represents a technological electrically inactive isoelectronic impurity. However, under various technological treatments (thermal treatment, irradiation), carbon effectively interacts with structural defects forming electrically active complexes that considerably affect the parameters of materials and devices produced on their basis. The properties of carbon in silicon both in grown crystals and after thermal and radiation treatments have been widely investigated during several decades [1 13]. But, in spite of intensive studies, there still remain a lot of unsolved problems concerning the influence of carbon on the processes of thermal and radiationinduced defect formation. The obtaining of new information on properties of carbon is important both from the fundamental viewpoint and from the practical one, as carbon doping is widely used today in nanotechnologies, for example for the production of Si:Ge relaxed layers on Si. Under irradiation, selfinterstitials push carbon from sites to interstices according to the Watkins exchange mechanism [3], which results in the formation of a stable defect (C i ). It is annealed out by diffusion at temperatures close to room one (T 310 K). In the course of diffusion in the lattice, interstitial carbon effectively interacts with impurities forming a large variety of electrically active defects of the interstitial kind. In silicon grown by the Czochralski method, the defect C i effectively interacts with interstitial oxygen (O i ), substitution carbon (C s ), selfinterstitials (Si i ), and impurities of groups III or V, which results in the formation of C i O i, C i C s, C i Si i, and C i +(III, V) s complexes, respectively [4 6,12,13]. It was recently found out that C i in silicon effectively interacts with atoms of isoelectronic tin and germanium impurities with formation of C i Sn s and C i Ge s stable complexes [14 19], though C i, Sn, and Ge form deformations of the same sign in the silicon lattice. The possibility of interaction of interstitial carbon with various sinks in the silicon lattice was widely discussed in literature, though the available data are ambiguous. For example, according to [6], the ratio of the radii of capture of C i by interstitial oxygen and onsite carbon that determine the possibilities of interaction amounts to 0.3, whereas in [8] this ratio is equal to 3. There are no data on the efficiency of interaction of C i with atoms of Sn and Ge isoelectronic impurities in silicon attracting heightened interest due to the development of materials for producing fast acting devices. This work is devoted to the study of the comparative efficiency of interaction of interstitial carbon with substitution carbon, oxygen, and tin atoms. Investigations of the efficiency of interaction of interstitial carbon with various sinks are important for the development of the control influence on the defect composition of a material, as defects formed with participation of C i atoms are electrically active and substantially affect the electrophysical properties of silicon. 222 ISSN Ukr. J. Phys Vol. 55, No. 2
2 EFFICIENCY OF INTERACTION OF INTERSTITIAL CARBON 2. Samples and Experimental Technique We investigated singlecrystal samples of ntype (phosphorusdoped) silicon grown using the Czochralski method. The phosphorus concentration was determined measuring the Hall effect and equaled (2 3) cm 3. The tin content in Si:Sn was determined by means of the neutronactivation analysis as well as with the help of a JCXA733 Xray microanalyzer. The concentrations of oxygen and carbon were found based on the intensities of the 1107cm 1 and 607cm 1 absorption lines, respectively [11, 20]. The parameters of the investigated samples are given in Table. The samples were irradiated by 5MeV electrons at a temperature close to 90 K using an М30 microtron. The irradiation dose amounted to cm 2. The efficiencies of interaction of interstitial carbon with impurities were determined based on the isochronous (20minute) annealing of the irradiated samples in the temperature range K at a step of 10 K. The absorption spectra of the samples were investigated with the help of an IFS113v Fourier spectrometer. The measurements were performed at a temperature of 10 K with a 0.5cm 1 resolution. 3. Experimental Results and Their Analysis 3.1. Interaction of C i with interstitial oxygen and substitution carbon As is known, the main sinks for interstitial carbon diffusing under annealing in Czochralski silicon are interstitial oxygen and substitutional carbon resulting in the formation of С i O i and С i C s complexes, respectively. The efficiency of formation of these complexes is proportional to the concentrations of the interacting components. Therefore, if the oxygen concentration (N O ) considerably exceeds that of carbon (N C ), the main trap for С i will be oxygen; while, under the condition N C N O, interstitial carbon will interact more effectively with C s. The oxygen concentration in Czochralski silicon is often Concentrations of tin, oxygen, and carbon in the samples Sample N Sn, cm 3 N O, cm 3 N C, cm 3 Si Si:Sn Si:Sn Si:Sn Si:Sn Fig. 1. Transformation of the absorption spectrum under annealing of electronirradiated Si at T ann = 250 (1 ), 287 (2 ), and 305 K (3 ). Φ e= cm 2, N O = cm 3, N C = cm 3 either larger than the content of carbon or close to it. In the latter case, there occurs the competitive interaction of С i with the both impurities. In order to estimate the probabilities of the interaction of С i with O i and C s, we used samples with close initial concentrations of oxygen and carbon (see Table). Figure 1 shows the absorption spectrum registered at 10 K for a sample irradiated at T 90 K by the dose Φ e = cm 2 and annealed to 250 K, as well as its transformation after the following annealing of interstitial carbon. As one can see from Fig. 1, the spectrum at T ann =250 K (curve 1) contains intense absorption lines with frequencies of 922, 932, and 6903 cm 1 corresponding to interstitial carbon [6]. Less intense lines with frequencies equal to 960 and 966 cm 1 correspond to C i Si i centers [12]. Under the annealing of С i (curves 2 and 3), there synchronously appear the lines corresponding to С i O i (865.9 cm 1 ) and С i C s ( cm 1 ) complexes [4 6]. The temperature of the complete annealing of С i is close to 305 K. Based on the obtained data on the intensities of the absorption lines corresponding to С i O i and С i C s complexes (865.9 and cm 1 ), we determined their concentrations using the coefficients and cm 2, respectively [6,21]. Our estimates show that the concentration of С i O i is equal to cm 3, whereas that of С i C s amounts to cm 3. ISSN Ukr. J. Phys Vol. 55, No
3 M.I. GRITSENKO, O.O. KOBZAR, Yu.V. POMOZOV et al. Fig. 3. Relative change of the concentration of interstitial carbon under the isochronous annealing of irradiated Si:Sn crystals. N Sn = 0 (1 ), (2 ), (3 ), (4 ), and cm 3 (5 ) Fig. 2. Transformation of the absorption spectrum under the annealing of electronirradiated Si:Sn at T ann = 240 (1 ), 260 (2 ), 305 (3 ), and 380 K (4 ). Φ e= cm 2. N Sn = cm 3, N C = cm 3 Thus, the obtained results testify to the fact that the concentrations of the both centers are comparable, i.e. the ratio of the probabilities of their formation is close to 1, rather than to 0.3 as in [6] or 3 as in [8]. It is worth noting that the concentrations of С i O i and С i C s complexes available in the literature were usually estimated at room annealing temperature after the complete vanishing of interstitial carbon. In [22], it was shown that, in the case of the complete annealing of С i centers, the concentration of С i O i complexes did not reach a maximum, as a considerable portion of С i was a part of the socalled precursors of С i O i that transformed into a stable С i O i configuration as the temperature increased to 340 K. The ratio of the С i O i and С i C s concentrations estimated from the obtained experimental data for the samples annealed to T ann = 340 K amounts to Interaction of C i with tin Another effective sink for interstitial carbon in silicon is tin [14 18], though its covalent radius (1.44 Å) is larger than the radius of the matrix (1.17 Å), and it effectively interacts with vacancies [2]. Figure 2 presents the transformation of the absorption spectrum for Si:Sn (curve 1) under the isochronous annealing in the temperature range K. As one can see from Fig. 2, in the case of the annealing of interstitial carbon (T ann > 250 K) in Si:Sn, one does not observe the absorption lines corresponding to С i O i and С i C s that were registered in Si. Instead, there appear six absorption lines corresponding to C i Sn complexes. According to [16 18], the lines with frequencies of 888.9, 985.3, and 6915 cm 1 correspond to a less stable configuration of the given centers and are annealed at T ann 280 K, whereas the lines at 873.5, , and 6875 cm 1 correlate with a more stable configuration and are annealed at T ann 380 K. A considerable intensification of the lines corresponding to C i O i and C i C s centers in Si:Sn is observed only in the case of the annealing of C i Sn complexes in the temperature range T ann = K. Figure 3 shows the intensities of the absorption lines corresponding to C i versus the annealing temperature for Si (curve 1) and Si:Sn (curves 2 5) plotted with the use of the results obtained in the course of isochronous annealing of the irradiated samples. As one can see from the figure, interstitial carbon in tindoped Si is less thermostable than that in Si. The larger the content of Sn in the samples, the lower the initial annealing temperature of C i. For example, at N Sn = cm 3, the annealing begins at T ann 255 K, while at N Sn = cm 3 at T ann 245 K. The figure also demonstrates that, as compared to silicon, the tem 224 ISSN Ukr. J. Phys Vol. 55, No. 2
4 EFFICIENCY OF INTERACTION OF INTERSTITIAL CARBON perature of the complete annealing of С i considerably decreases with increasing the tin content. We estimated the efficiency of the capture of diffusing С i by Sn impurity atoms as compared to the probabilities of the capture by such sinks as O i and C s. The results of measurements could not be directly used for such estimations, as the investigated Si:Sn samples contained different concentrations of carbon, whereas the formation of C i O i and C i C s complexes under the annealing of C i was registered only in one sample with the minimal Sn content. That is why the efficiency of the capture of С i by Sn atoms was estimated using the approximation of quasichemical reactions [23]. As is known, the annealing of interstitial carbon in silicon can be described by the following reactions [4 6]: C i + O i C i O i, (1) C i + C s C i C s. (2) In the presence of tin, the following reaction also takes place: C i + Sn s C i Sn. (3) With regard for reactions (1) (3), the process of annealing of C i in Si:Sn crystals can be described by the kinetic equation dn Ci dt = χ Ci, O i N Ci N Oi χ Ci, C s N Ci N Cs χ Ci, SnN Ci N Sn, (4) where N denote the concentrations of the interacting defects, and χ are the probabilities of reactions between the corresponding components. In [23, 24], it was shown that, under the annealing of defects by means of diffusion to immovable sinks, the probabilities of reactions χ can be presented in the form ( χ = 4πD 0 exp E ) a r, (5) kt where Е a is the diffusion activation energy, k is the Boltzmann constant, Т is the absolute temperature, r is the effective radius of capture of a diffusing component by a sink, and D 0 = zν 0 l 2, where z is an integer depending on the type of the crystal lattice, ν 0 is the frequency of thermal oscillations, and l is the interatomic distance. In view of (5), Eq. (4) can be presented in the form ( dn Ci = 4πD 0 exp E ) a N Ci r Ci, mn m, (6) dt kt where N m are the concentrations of the corresponding sinks. In order to perform the further analysis of Eq. (6), it is necessary to establish the explicit time dependence of the annealing temperature T = f(t). As the temperature changes stepwise, it is appropriate to use the linear approximation [25] T = T 0 + at, (7) where a = ΔT/Δt is the mean rate of increase of the annealing temperature. According to [25], approximation (7) practically has no effect on the final result if the rate a remains constant in the annealing process. Integrating Eq. (6) after the change of variables (7), we obtain ln N C i = 4πD ( 0k T 2 exp E ) a r Ci, mn m, (8) ae a kt N Ci(0) where N Ci(0) is the initial concentration of С i, and N Ci is the concentration of С i after the annealing to some temperature Т. In what follows, the annealing temperature of interstitial carbon Т a will mean such a temperature, at which the concentration of the given centers decreases by a factor of е with respect to the initial value. Under / the condition T = T a, we obtain the equality N Ci NCi(0) = e 1. As a result, Eq. (8) yields Ta 2 ( exp E ) a a r Ci, mn m = E a kt a 4πD m 0 k. (9) Equation (9) establishes the relationship between such parameters as the annealing temperature of С i, the diffusion activation energy of a given center Е a, and the sink concentration N m with regard for the corresponding capture radii. Using the results of isochronous annealing of the investigated crystals, we estimated the diffusion activation energy of C i in samples with various tin contents according to the technique described in [25]. Our estimates demonstrate that, at the considered concentrations of tin in Si, the activation energy takes the value Е a = (0.75±0.02) ev which insignificantly differs from the known annealing activation energy of C i in Si that amounts to 0.77 ev [10]. m m ISSN Ukr. J. Phys Vol. 55, No
5 M.I. GRITSENKO, O.O. KOBZAR, Yu.V. POMOZOV et al. Estimating the efficiencies of the interaction of interstitial carbon with Sn impurity atoms, we allowed for the fact that the probabilities of their capture by such sinks as O i and C s are equal, as was demonstrated above. Then, with regard for the concentrations of the impurities and the experimentally determined annealing temperatures of С i in Si:Sn samples, using Eq. (9) and the energy Е a, we derived the following relation for the radii of capture of С i by O i, C s, and Sn sinks: r Ci, O i : r Ci, C s : r Ci, Sn s 1 : 1 : 2.3. (10) In view of (5), the same relation can be written for the corresponding probabilities of the reactions: χ Ci, O i : χ Ci, C s : χ Ci, Sn s 1 : 1 : 2.3. (11) Using relation (11) and taking values of the contents of the tin, oxygen, and carbon impurities from Table, we estimated the concentrations of С i Sn, C i O i, and C i C s complexes formed at the annealing of С i in the investigated samples. It was found that, in the sample with the minimal tin content N Sn = cm 3 at the corresponding concentrations of oxygen and carbon, the resulting concentration of С i Sn centers exceeded that of C i O i and C i C s complexes more than by a factor of five. In the sample with the maximal tin concentration N Sn = cm 3, this ratio already reaches fifty. These estimates give a possibility to explain the fact that, after the annealing of C i in samples with a large tin content, the absorption spectra practically do not contain bands corresponding to C i O i and C i C s complexes. 4. Conclusions We studied the efficiencies of the interaction of interstitial carbon with the basic technological impurities in silicon, oxygen and substitutional carbon, as well as with an isoelectronic impurity, tin. It is shown that the probabilities of the interaction of interstitial carbon with interstitial oxygen and substitution carbon in the silicon lattice are close. It is found that interstitial carbon in tindoped Si is less thermostable as compared with silicon, and the temperature of its complete annealing gradually decreases with increasing the tin concentration. The probabilities of the capture of diffusing С i atoms by O i, C s, and Sn impurity atoms are quantitatively estimated. It is shown that the probability of the interaction of С i with tin is higher than the probability of its interaction with oxygen and substitution carbon by a factor of 2.3. We also estimated the concentrations of С i Sn, C i O i, and C i C s complexes formed in the investigated samples under the annealing of С i with regard for the content of oxygen, carbon, and tin in the initial samples (see Table). Our estimates demonstrate that the concentration of С i Sn centers in the Si:Sn1 sample with the minimal tin concentration (N Sn = cm 3 ) is higher than that of C i O i and C i C s centers by a factor of five, whereas, for the Si:Sn4 sample (N Sn = ) cm 3, this ratio reaches fifty. 1. A. Brelot and J. Charlemagne, in Radiation Effects in Semiconductors, ed. by J.W. Corbett and G.D. Watkins (Gordon and Breach, London, 1971), p G.D. Watkins, Phys. Rev. B 12, 4383 (1975). 3. G.D. Watkins and K.L. Brower, Phys. Rev. Lett. 36, 1329 (1976). 4. A.B. Bean, R.C. Newman, and R.S. Smith, J. Phys. Chem. Solids 31, 739 (1970). 5. J.M. Trombetta and G.D. Watkins, Appl. Phys. Lett. 51, 1103 (1987). 6. G. Davies, A.S. Oates, R.C. Newman, R. Woolley, E.C. Lightowlers, M.J. Binns, and J.L. Wilkes, J. Phys. C: Sol. State Phys. 19, 841 (1986). 7. B.G. Svensson, J. Svensson, J.L. Lindström, G. Davies, and J.M. Corbett, Appl. Phys. Lett. 51, 2257 (1987). 8. V.P. Markevich and L.I. Murin, Fiz. Tekhn. Polupr. 22, 911 (1988). 9. G. Davies, Mater. Sci. Forum, 3841, 151 (1989). 10. L.W.Song and G.D. Watkins, Phys. Rev. B 42, 5759 (1990). 11. G. Davies and R.C. Newman, Handbook on Semiconductors, ed. by T.S. Moss (Elsevier, Amsterdam, 1994) and references therein. 12. L.I. Murin, J.L. Lindström, G. Davies, and V.P. Markevich, Nucl. Instr. Meth. Phys. Res. B 253, 210 (2006). 13. M.T. Asom, J.L. Benton, R. Sauer, and L.C. Kimerling, Appl. Phys. Lett. 51, 256 (1987). 14. E.V. Lavrov and M. Fanciulli, Physica B , 263 (2001). 15. E.V. Lavrov, M. Fanciulli, M. Kaukonen, R. Jones, and P.R. Briddon, Phys. Rev. B 64, (2001). 16. L.I. Khirunenko, O.A. Kobzar, Yu.V. Pomozov, M.G. Sosnin, and N.A. Tripachko, Fiz. Tekhn. Polupr. 37, 304 (2003). 17. L.I. Khirunenko, O.O. Kobzar, Yu.V. Omozov, M.G. Sosnin, M.O. Tripachko, N.V. Abrosimov, and H. Riemann, Physica B , 546 (2003). 18. L.I. Khirunenko, O.O. Kobzar, Yu.V. Pomozov, M.G. Sosnin, M.O. Tripachko, N.V. Abrosimov, and H. Riemann, Sol. State Phenom , 393 (2004). 226 ISSN Ukr. J. Phys Vol. 55, No. 2
6 EFFICIENCY OF INTERACTION OF INTERSTITIAL CARBON 19. L.I. Khirunenko, Yu.V. Pomozov, M.G. Sosnin, A. Duvanskii, V.J.B. Torres, J. Coutinho, R. Jones, P.R. Briddon, N.V. Abrosimov, and H. Riemann, Physica B: Cond. Matter, , 200 (2007). 20. A. Baghadadi, W.M. Bullis, M.C. Choarkin, L. Yuezhen, R.I. Scace, R.W. Series, P. Stallhofer, and M. Watanable, J. Electrochem. Soc. 136, 2015 (1989). 21. E.V. Lavrov, L. Hoffmann, and B. BechNielsen, Phys. Rev. B 60, 8081 (1999). 22. V.L. Vinetskii and G.A. Kholodar, Radiation Physics of Semiconductors (Naukova Dumka, Kiev, 1979) (in Russian). 23. V.V. Emtsev and T.V. Mashovets, Impurities and Point Defects in Semiconductors (Radio i Svyaz, Moscow, 1981) (in Russian). 24. J. Bourgion and M. Lanno, Point Defects in Semiconductors. Experimental Aspects (Springer, Berlin, 1983). Received Translated from Ukrainian by H.G. Kalyuzhna ЕФЕКТИВНIСТЬ ВЗАЄМОДIЇ МIЖВУЗЛОВИННОГО ВУГЛЕЦЮ З КИСНЕМ, ОЛОВОМ I ВУГЛЕЦЕМ ЗАМIЩЕННЯ В ОПРОМIНЕНОМУ КРЕМНIЇ М.I. Гриценко, О.О. Кобзар Ю.В. Помозов, М.Г. Соснiн, Л.I. Хируненко Р е з ю м е У роботi методом iнфрачервоної фур єспектроскопiї проведено дослiдження ефективностi взаємодiї мiжвузловинного вуглецю з основними технологiчними домiшками кремнiю киснем та вуглецем замiщення, а також з iзоелектронною домiшкою оловом. Показано, що ймовiрностi взаємодiї мiжвузловинного вуглецю з мiжвузловинним киснем та вузловим вуглецем є близькими за величиною. Виявлено, що мiжвузловинний вуглець у Si, легованому оловом, має меншу термiчну стабiльнiсть, нiж у кремнiї, i температура його остаточного вiдпалу поступово знижується при зростаннi концентрацiї олова. Показано, що ймовiрнiсть взаємодiї мiжвузловинного вуглецю з оловом у 2,3 раза перевищує ймовiрнiсть його взаємодiї з киснем та вузловим вуглецем. ISSN Ukr. J. Phys Vol. 55, No
Ch. 4: Imperfections in Solids Part 1. Dr. Feras Fraige
Ch. 4: Imperfections in Solids Part 1 Dr. Feras Fraige Outline Defects in Solids 0D, Point defects vacancies Interstitials impurities, weight and atomic composition 1D, Dislocations edge screw 2D, Grain
More informationChapter 5: Diffusion. 5.1 SteadyState Diffusion
: Diffusion Diffusion: the movement of particles in a solid from an area of high concentration to an area of low concentration, resulting in the uniform distribution of the substance Diffusion is process
More informationChapter Outline. Diffusion  how do atoms move through solids?
Chapter Outline iffusion  how do atoms move through solids? iffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities The mathematics of diffusion Steadystate diffusion (Fick s first law)
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationAnnealing behaviour of plastically deformed stainless steel 1.4307 studied by positron annihilation methods
NUKLEONIKA 2013;58(1):215 219 ORIGINAL PAPER Annealing behaviour of plastically deformed stainless steel 1.4307 studied by positron annihilation methods Ewa Dryzek, Maciej Sarnek, Krzysztof Siemek Abstract.
More informationMaterials Science and Engineering Department MSE , Sample Test #1, Spring 2010
Materials Science and Engineering Department MSE 200001, Sample Test #1, Spring 2010 ID number First letter of your last name: Name: No notes, books, or information stored in calculator memories may be
More informationSolid State Detectors = SemiConductor based Detectors
Solid State Detectors = SemiConductor based Detectors Materials and their properties Energy bands and electronic structure Charge transport and conductivity Boundaries: the pn junction Charge collection
More informationIn order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 103 m. Thus,
5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS
41 CHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and SelfInterstitials 4.1 In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation
More informationTDS. Dirk Rosenthal Department of Inorganic Chemistry FritzHaberInstitut der MPG Faradayweg 46, DE 14195 Berlin dirkrose@fhiberlin.mpg.
Modern Methods in Heterogeneous Catalysis Research TDS Dirk Rosenthal Department of Inorganic Chemistry FritzHaberInstitut der MPG Faradayweg 46, DE 14195 Berlin dirkrose@fhiberlin.mpg.de TDS = TPD
More informationThe plasmoelectric effect: optically induced electrochemical potentials in resonant metallic structures
The plasmoelectric effect: optically induced electrochemical potentials in resonant metallic structures Matthew T. Sheldon and Harry A. Atwater Thomas J. Watson Laboratories of Applied Physics, California
More informationDoped Semiconductors. Dr. Katarzyna Skorupska
Doped Semiconductors Dr. Katarzyna Skorupska 1 Doped semiconductors Increasing the conductivity of semiconductors by incorporation of foreign atoms requires increase of the concentration of mobile charge
More informationCHEM 10113, Quiz 7 December 7, 2011
CHEM 10113, Quiz 7 December 7, 2011 Name (please print) All equations must be balanced and show phases for full credit. Significant figures count, show charges as appropriate, and please box your answers!
More information7. DYNAMIC LIGHT SCATTERING 7.1 First order temporal autocorrelation function.
7. DYNAMIC LIGHT SCATTERING 7. First order temporal autocorrelation function. Dynamic light scattering (DLS) studies the properties of inhomogeneous and dynamic media. A generic situation is illustrated
More informationAnharmonicity and Weak Mode Assignment in La 2 x Sr x CuO 4 with Oxygen Isotopic Substitution
Vol. 111 (2007) ACTA PHYSICA POLONICA A No. 1 Proceedings of the Symposium K: Complex Oxide Materials for New Technologies of EMRS Fall Meeting 2006, Warsaw, September 4 8, 2006 Anharmonicity and Weak
More informationIntroduction To Materials Science FOR ENGINEERS, Ch. 5. Diffusion. MSE 201 Callister Chapter 5
Diffusion MSE 21 Callister Chapter 5 1 Goals: Diffusion  how do atoms move through solids? Fundamental concepts and language Diffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities Diffusion
More informationChapter Outline. Defects Introduction (I)
Crystals are like people, it is the defects in them which tend to make them interesting!  Colin Humphreys. Defects in Solids Chapter Outline 0D, Point defects vacancies interstitials impurities, weight
More informationJournal of the University of Chemical Technology and Metallurgy, 42, 2, 2007. 2) are in C 1
Journal of the University of Chemical M. Georgiev, Technology D. Stoilova and Metallurgy, 42, 2, 2007, 211216 METALWATER INTERACTINS AND HYDRGEN BND STRENGTH M. Georgiev 1, D. Stoilova 2 1 University
More informationThe study of deeplevel emission center in ZnO films grown on cal 2 O 3 substrates
The study of deeplevel emission center in ZnO films grown on cal 2 O 3 substrates Guotong Du Yuantao Zhang, Jinzhong Wang, Yongguo Cui (College of Electronic Science and Engineering, State Key Laboratory
More information3. What would you predict for the intensity and binding energy for the 3p orbital for that of sulfur?
PSI AP Chemistry Periodic Trends MC Review Name Periodic Law and the Quantum Model Use the PES spectrum of Phosphorus below to answer questions 13. 1. Which peak corresponds to the 1s orbital? (A) 1.06
More informationINSTITUTE FOR APPLIED PHYSICS Physical Practice for Learners of Engineering sciences Hamburg University, Jungiusstraße 11
INSTITUTE FOR APPIED PHYSICS Physical Practice for earners of Engineering sciences Hamburg University, Jungiusstraße 11 Hall effect 1 Goal Characteristic data of a test semiconductor (Germanium) should
More informationThe impact of Secontent on the optical properties of CuInSe 2 by using transmittance and photoacoustic spectroscopies
The impact of Secontent on the optical properties of CuInSe 2 by using transmittance and photoacoustic spectroscopies * Fatima Zohra Satour and Ameur Zegadi LCCNS, Département d Electronique, Faculté
More informationTHE WAY TO SOMEWHERE. Subtopics. Diffusion Diffusion processes in industry
THE WAY TO SOMEWHERE Subtopics 1 Diffusion Diffusion processes in industry RATE PROCESSES IN SOLIDS At any temperature different from absolute zero all atoms, irrespective of their state of aggregation
More informationThe Physics of Energy sources Renewable sources of energy. Solar Energy
The Physics of Energy sources Renewable sources of energy Solar Energy B. Maffei Bruno.maffei@manchester.ac.uk Renewable sources 1 Solar power! There are basically two ways of using directly the radiative
More informationphys4.17 Page 1  under normal conditions (pressure, temperature) graphite is the stable phase of crystalline carbon
Covalent Crystals  covalent bonding by shared electrons in common orbitals (as in molecules)  covalent bonds lead to the strongest bound crystals, e.g. diamond in the tetrahedral structure determined
More informationUltraviolet laser removal of small metallic particles from silicon wafers
Optics and Lasers in Engineering 38 (2002) 405 415 Ultraviolet laser removal of small metallic particles from silicon wafers C. Curran a, *, J.M. Lee b, K.G. Watkins a a Laser Group, Department of Engineering,
More informationChem 115 POGIL Worksheet  Week 4 Moles & Stoichiometry
Chem 115 POGIL Worksheet  Week 4 Moles & Stoichiometry Why? Chemists are concerned with mass relationships in chemical reactions, usually run on a macroscopic scale (grams, kilograms, etc.). To deal with
More informationPublication VI. c 2012. Reprinted with permission.
Publication VI C. Rauch, F. Tuomisto, P. D. C. King, T. Veal, H. Lu, and W. J. Schaff. Selfcompensation in highly ntype InN. arxiv:1204.3299v1 [condmat.mtrlsci], pages 1 5, April 2012. c 2012. Reprinted
More informationTypes of Epitaxy. Homoepitaxy. Heteroepitaxy
Epitaxy Epitaxial Growth Epitaxy means the growth of a single crystal film on top of a crystalline substrate. For most thin film applications (hard and soft coatings, optical coatings, protective coatings)
More informationHigh Open Circuit Voltage of MQW Amorphous Silicon Photovoltaic Structures
High Open Circuit Voltage of MQW Amorphous Silicon Photovoltaic Structures ARGYRIOS C. VARONIDES Physics and EE Department University of Scranton 800 Linden Street, Scranton PA, 18510 United States Abstract:
More informationDIFFUSION IN SOLIDS. Materials often heat treated to improve properties. Atomic diffusion occurs during heat treatment
DIFFUSION IN SOLIDS WHY STUDY DIFFUSION? Materials often heat treated to improve properties Atomic diffusion occurs during heat treatment Depending on situation higher or lower diffusion rates desired
More informationMOLECULAR DYNAMICS INVESTIGATION OF DEFORMATION RESPONSE OF THINFILM METALLIC NANOSTRUCTURES UNDER HEATING
NANOSYSTEMS: PHYSICS, CHEMISTRY, MATHEMATICS, 2011, 2 (2), P. 76 83 UDC 538.97 MOLECULAR DYNAMICS INVESTIGATION OF DEFORMATION RESPONSE OF THINFILM METALLIC NANOSTRUCTURES UNDER HEATING I. S. Konovalenko
More informationSpectroscopy. The Interaction of Electromagnetic Radiation (Light) with Molecules
Spectroscopy. The Interaction of Electromagnetic Radiation (Light) with Molecules (1) Electromagnetic Radiationwave description propagation c = 3 x 10 10 cm/sec magnetic () and electric (E) field vectors
More informationELECTRICAL, ACOUSTIC AND ACOUSTOOPTICAL PROPERTIES OF Si (Ge) Se Te GLASSES
Chalcogenide Letters Vol. 2, No. 9, September 2005, p. 8391 ELECTRICAL, ACOUSTIC AND ACOUSTOOPTICAL PROPERTIES OF Si (Ge Se Te GLASSES L. A. Kulakova, V. Kh. Kudoyarova *, B. T. Melekh and V. I. Bakharev
More informationEffect of energy scale imperfections on results of neutrino mass measurements from βdecay
Effect of energy scale imperfections on results of neutrino mass measurements from βdecay J. Kašpar 1, M. Ryšavý, A. Špalek and O. Dragoun Nuclear Physics Institute, Acad. Sci. Czech Rep., CZ 250 68 Řež
More informationSEMICONDUCTOR I: Doping, semiconductor statistics (REF: Sze, McKelvey, and Kittel)
SEMICONDUCTOR I: Doping, semiconductor statistics (REF: Sze, McKelvey, and Kittel) Introduction Based on known band structures of Si, Ge, and GaAs, we will begin to focus on specific properties of semiconductors,
More informationThermal transport in the anisotropic Heisenberg chain with S = 1/2 and nearestneighbor interactions
Thermal transport in the anisotropic Heisenberg chain with S = 1/2 and nearestneighbor interactions D. L. Huber Department of Physics, University of WisconsinMadison, Madison, WI 53706 Abstract The purpose
More informationElectrical Conductivity
Advanced Materials Science  Lab Intermediate Physics University of Ulm Solid State Physics Department Electrical Conductivity Translated by MichaelStefan Rill January 20, 2003 CONTENTS 1 Contents 1 Introduction
More informationSemiconductor Physics
10p PhD Course Semiconductor Physics 18 Lectures NovDec 2011 and Jan Feb 2012 Literature Semiconductor Physics K. Seeger The Physics of Semiconductors Grundmann Basic Semiconductors Physics  Hamaguchi
More informationFUNDAMENTAL PROPERTIES OF SOLAR CELLS
FUNDAMENTAL PROPERTIES OF SOLAR CELLS January 31, 2012 The University of Toledo, Department of Physics and Astronomy SSARE, PVIC Principles and Varieties of Solar Energy (PHYS 4400) and Fundamentals of
More informationTopic 3 Periodic Trends
Topic 3 Periodic Trends Chapter 06 Trends on the Periodic Table Chapter 07 Relationships between the elements CHEM 10 T03D01 How are elements arranged Prior to 1735, only 12 elements were known to man
More informationChem 115 POGIL Worksheet  Week 4 Moles & Stoichiometry Answers
Key Questions & Exercises Chem 115 POGIL Worksheet  Week 4 Moles & Stoichiometry Answers 1. The atomic weight of carbon is 12.0107 u, so a mole of carbon has a mass of 12.0107 g. Why doesn t a mole of
More informationPrussian blue nanoparticles for laserinduced photothermal therapy of tumors
Electronic Supplementary Material (ESI) for RSC Advances. This journal is The Royal Society of Chemistry 2014 Supporting Information Prussian blue nanoparticles for laserinduced photothermal therapy of
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationElectron spectroscopy Lecture 121. Kai M. Siegbahn (1918  ) Nobel Price 1981 High resolution Electron Spectroscopy
Electron spectroscopy Lecture 121 Kai M. Siegbahn (1918  ) Nobel Price 1981 High resolution Electron Spectroscopy 653: Electron Spectroscopy urse structure cture 1. Introduction to electron spectroscopies
More informationCHARACTERIZATION AND MODELING OF STRESS EVOLUTION DURING NICKEL SILICIDES FORMATION
CHARACTERIZATION AND MODELING OF STRESS EVOLUTION DURING NICKEL SILICIDES FORMATION K. P. LIEW 1, Y. LI, M. YEADON 3, R. BERNSTEIN 4, C. V. THOMPSON 4 1 SingaporeMIT Alliance, Advanced Materials for Micro
More informationChapter 8. Low energy ion scattering study of Fe 4 N on Cu(100)
Low energy ion scattering study of 4 on Cu(1) Chapter 8. Low energy ion scattering study of 4 on Cu(1) 8.1. Introduction For a better understanding of the reconstructed 4 surfaces one would like to know
More informationChapter 5. Second Edition ( 2001 McGrawHill) 5.6 Doped GaAs. Solution
Chapter 5 5.6 Doped GaAs Consider the GaAs crystal at 300 K. a. Calculate the intrinsic conductivity and resistivity. Second Edition ( 2001 McGrawHill) b. In a sample containing only 10 15 cm 3 ionized
More informationLecture 8: Extrinsic semiconductors  mobility
Lecture 8: Extrinsic semiconductors  mobility Contents Carrier mobility. Lattice scattering......................... 2.2 Impurity scattering........................ 3.3 Conductivity in extrinsic semiconductors............
More information14:635:407:02 Homework III Solutions
14:635:407:0 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 37 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More informationSUPERCONDUCTIVITY. PH 318 Introduction to superconductors 1
SUPERCONDUCTIVITY property of complete disappearance of electrical resistance in solids when they are cooled below a characteristic temperature. This temperature is called transition temperature or critical
More informationMechanisms of Diffusion in Materials 3.205 L4 11/7/06
Mechanisms of Diffusion in Materials 1 A final point on interdiffusion The composition profiles resulting from interdiffusion are generally constrained by phase equilibria. Consider the an Ir Re diffusion
More informationThermal Behavior of Al and In Impurities Doped in ZnO Studied by Means of Perturbed Angular Correlation Spectroscopy
Title Author(s) Thermal Behavior of Al and In Impur of Perturbed Angular Correlation Sp 小 松 田, 沙 也 加 Citation 博 士 論 文 要 旨 Abstract Issue Date 20150323 Type Thesis or Dissertation Text version none URL
More informationDefect Engineering in Semiconductors
Defect Engineering in Semiconductors Silicon Technology: problems of ultra largescale l integration i Gettering in silicon Defect engineering in HgCdTe Nearsurface defects in GaAs after diamond sawcutting
More informationElectronic Structure and the Periodic Table Learning Outcomes
Electronic Structure and the Periodic Table Learning Outcomes (a) Electronic structure (i) Electromagnetic spectrum and associated calculations Electromagnetic radiation may be described in terms of waves.
More information8. Kinetic Monte Carlo
8. Kinetic Monte Carlo [Duane Johnsons notes in web; Per Stoltze: Simulation methods in atomicscale physics; Fichthorn, Weinberg: J. Chem. Phys. 95 (1991) 1090; Bortz, Kalos, Lebowitz, J. Computational
More informationCharacteristic curves of a solar cell
Related Topics Semiconductor, pn junction, energyband diagram, Fermi characteristic energy level, diffusion potential, internal resistance, efficiency, photoconductive effect, acceptors, donors, valence
More informationThe General Properties of Si, Ge, SiGe, SiO 2 and Si 3 N 4 June 2002
The neral Properties of,,, O 2 and 3 N 4 June 2002 Virginia Semiconductor 1501 Powhatan Street, Fredericksburg, VA 224014647 USA Phone: (540) 3732900, FAX (540) 3710371 www.virginiasemi.com, tech@virginiasemi.com
More informationInfrared Spectroscopy: Theory
u Chapter 15 Infrared Spectroscopy: Theory An important tool of the organic chemist is Infrared Spectroscopy, or IR. IR spectra are acquired on a special instrument, called an IR spectrometer. IR is used
More informationSolar Cell Parameters and Equivalent Circuit
9 Solar Cell Parameters and Equivalent Circuit 9.1 External solar cell parameters The main parameters that are used to characterise the performance of solar cells are the peak power P max, the shortcircuit
More informationSemiconductor Detectors Calorimetry and Tracking with High Precision
Semiconductor Detectors Calorimetry and Tracking with High Precision Applications 1. Photon spectroscopy with high energy resolution. Vertex detection with high spatial resolution 3. Energy measurement
More informationA System for Possible Early Warning of Disastrous Solar Flares
A System for Possible Early Warning of Disastrous Solar Flares Jere Jenkins Ephraim Fischbach 116m In Decay 500 450 400 350 y = 0.000203x + 6.044443 R 2 = 0.980358 7 6 5 Counts/10s 300 250 200 4 3 ln(counts/10s)
More informationCHAPTER  45 SEMICONDUCTOR AND SEMICONDUCTOR DEVICES
1. f = 101 kg/m, V = 1 m CHAPTER  45 SEMCONDUCTOR AND SEMCONDUCTOR DEVCES m = fv = 101 1 = 101 kg No.of atoms = 101 10 6 10 = 64.6 10 6. a) Total no.of states = N = 64.6 10 6 = 58.5 = 5. 10 8 10 6 b)
More informationNuclear ZPE Tapping. Horace Heffner May 2007
ENERGY FROM UNCERTAINTY The uncertainty of momentum for a particle constrained by distance Δx is given, according to Heisenberg, by: Δmv = h/(2 π Δx) but since KE = (1/2) m v 2 = (1/(2 m) ) (Δmv) 2 ΔKE
More informationEFFICIENCY FOR CLOSE GEOMETRIES AND EXTENDED SOURCES OF A PTYPE GERMANIUM DETECTOR WITH LOWENERGY SENSITIVITY.
Abstract EFFICIENCY FOR CLOSE GEOMETRIES AND EXTENDED SOURCES OF A PTYPE GERMANIUM DETECTOR WITH LOWENERGY SENSITIVITY R.M. Keyser (1) and T.R. Twomey (1) (1) ORTEC, 801 South Illinois Avenue, Oak Ridge,
More informationDevelopments in Photoluminescence Characterisation for Silicon PV
Developments in Photoluminescence Characterisation for Silicon PV School of Photovoltaic and Solar Energy Engineering Bernhard Mitchell 1, Thorsten Trupke 1,2, Jürgen W. Weber 2, Johannes Greulich 3, Matthias
More informationPTC Thermistors [From Philips Data Handbook PA ]
PTC Thermistors [From Philips Data Handbook PA02 1989] 1. GENERAL Positive Temperature Coefficient (PTC) thermistors exhibit a high positive temperature coefficient of resistance. They differ from Negative
More informationSPECTROSCOPIC STUDIES ON DEGRADATION OF POLY N,N'METHYLENE BISACRYLAMIDE
Int. J. Chem. Sci.: 8(4), 2010, 27952800 SPECTROSCOPIC STUDIES ON DEGRADATION OF POLY N,N'METHYLENE BISACRYLAMIDE V. SRIDHAR *, S. KALAHASTI a, B. SANJEEVA RAO b, S. INDIRA, K. GOPALA KISHAN RAO c and
More informationSteady Heat Conduction
Steady Heat Conduction In thermodynamics, we considered the amount of heat transfer as a system undergoes a process from one equilibrium state to another. hermodynamics gives no indication of how long
More informationDependence of the thickness and composition of the HfO 2 /Si interface layer on annealing
Dependence of the thickness and composition of the HfO 2 /Si interface layer on annealing CINVESTAVUNIDAD QUERETARO P.G. ManiGonzález and A. HerreraGomez gmani@qro.cinvestav.mx CINVESTAV 1 background
More informationSemiconductors, diodes, transistors
Semiconductors, diodes, transistors (Horst Wahl, QuarkNet presentation, June 2001) Electrical conductivity! Energy bands in solids! Band structure and conductivity Semiconductors! Intrinsic semiconductors!
More informationh e l p s y o u C O N T R O L
contamination analysis for compound semiconductors ANALYTICAL SERVICES B u r i e d d e f e c t s, E v a n s A n a l y t i c a l g r o u p h e l p s y o u C O N T R O L C O N T A M I N A T I O N Contamination
More informationLecture 2  Semiconductor Physics (I) September 13, 2005
6.012  Microelectronic Devices and Circuits  Fall 2005 Lecture 21 Lecture 2  Semiconductor Physics (I) September 13, 2005 Contents: 1. Silicon bond model: electrons and holes 2. Generation and recombination
More informationCarbon Cable. Sergio Rubio Carles Paul Albert Monte
Carbon Cable Sergio Rubio Carles Paul Albert Monte Carbon, Copper and Manganine PhYsical PropERTieS CARBON PROPERTIES Carbon physical Properties Temperature Coefficient α 0,0005 ºC1 Density D 2260 kg/m3
More informationPhase Characterization of TiO 2 Powder by XRD and TEM
Kasetsart J. (Nat. Sci.) 42 : 357361 (28) Phase Characterization of TiO 2 Powder by XRD and TEM Kheamrutai Thamaphat 1 *, Pichet Limsuwan 1 and Boonlaer Ngotawornchai 2 ABSTRACT In this study, the commercial
More informationHigh Stress Silicon Nitride Films for Strained Silicon Technology
High Stress Silicon Nitride Films for Strained Silicon Technology Bhadri Varadarajan*, Jim Sims PECVD Business Unit Novellus Systems, Inc. Effect of Strain on Carrier Mobility! Strain lifts degeneracy,
More informationPhysical Properties and Functionalization of LowDimensional Materials
Physical Properties and Functionalization of LowDimensional Materials Physics Department, University of Trieste Graduate School of Physics, XXVI cycle Supervisor: Cosupervisor: Prof. Alessandro BARALDI
More informationProject 2B Building a Solar Cell (2): Solar Cell Performance
April. 15, 2010 Due April. 29, 2010 Project 2B Building a Solar Cell (2): Solar Cell Performance Objective: In this project we are going to experimentally measure the IV characteristics, energy conversion
More informationLuminescence study of structural changes induced by laser cutting in diamond films
Luminescence study of structural changes induced by laser cutting in diamond films A. Cremades and J. Piqueras Departamento de Fisica de Materiales, Facultad de Fisicas, Universidad Complutense, 28040
More informationThe CVD diamond booklet
available at: www.diamondmaterials.com/download Content 1. General properties of diamond... 2 2. Optical Properties... 4 Optical transparency...4 Absorption coefficient at 10.6 µm...5 Refractive index:
More informationAnalyses on copper samples from Micans
PDF rendering: DokumentID 1473479, Version 1., Status Godkänt, Sekretessklass Öppen Analyses on copper samples from Micans P. Berastegui, M. Hahlin, M. Ottosson, M. Korvela, Y. Andersson, R. Berger and
More informationChapter 7 ( ) Second Edition ( 2001 McGrawHill) 7.1 Relative permittivity and polarizability. Solution. α e 4πε o r o
Chapter 7 Second Edition ( 2001 McGrawHill) 7.1 Relative permittivity and polarizability a. Show that the local field is given by E loc = E + 2 3 Local field b. Amorphous selenium (ase) is a high resistivity
More informationA reinterpretation of the phase transitions in Na 2 CO 3
Acta Crystallographica Section B Structural Science ISSN 01087681 Editor: Carolyn P. Brock A reinterpretation of the phase transitions in Na 2 CO 3 Alla Arakcheeva and Gervais Chapuis Copyright International
More informationSPACE CHARGE MEASUREMENTS IN XLPE INSULATED MID VOLTAGE CABLE: CORRELATION WITH CABLE PERFORMANCE
SPACE CHARGE MEASUREMENTS IN XLPE INSULATED MID VOLTAGE CABLE: CORRELATION WITH CABLE PERFORMANCE Idalberto TAMAYO, Univ. Politècnica de Catalunya (ETSEIAT), (Spain), jose.antonio.diego@upc.edu Jordi ÒRRIT,
More informationEach grain is a single crystal with a specific orientation. Imperfections
Crystal Structure / Imperfections Almost all materials crystallize when they solidify; i.e., the atoms are arranged in an ordered, repeating, 3dimensional pattern. These structures are called crystals
More informationPreface Light Microscopy Xray Diffraction Methods
Preface xi 1 Light Microscopy 1 1.1 Optical Principles 1 1.1.1 Image Formation 1 1.1.2 Resolution 3 1.1.3 Depth of Field 5 1.1.4 Aberrations 6 1.2 Instrumentation 8 1.2.1 Illumination System 9 1.2.2 Objective
More informationLecture 2: Semiconductors: Introduction
Lecture 2: Semiconductors: Introduction Contents 1 Introduction 1 2 Band formation in semiconductors 2 3 Classification of semiconductors 5 4 Electron effective mass 10 1 Introduction Metals have electrical
More informationEnergy Transport. Focus on heat transfer. Heat Transfer Mechanisms: Conduction Radiation Convection (mass movement of fluids)
Energy Transport Focus on heat transfer Heat Transfer Mechanisms: Conduction Radiation Convection (mass movement of fluids) Conduction Conduction heat transfer occurs only when there is physical contact
More informationLocal order measurement in SnGe alloys and monolayer Sn films on Si with reflection electron energy loss spectrometry
Local order measurement in SnGe alloys and monolayer Sn films on Si with reflection electron energy loss spectrometry Selmer S. Wong, Gang He, Shouleh Nikzad, a) Channing C. Ahn, and Harry A. Atwater Thomas
More informationSurface Parameters of Stannic Oxide in Powder, Ceramic and Gel Forms by Nitrogen Adsorption Techniques l
PHYSICAL SCIENCES 137 Surface Parameters of Stannic Oxide in Powder, Ceramic and Gel Forms by Nitrogen Adsorption Techniques l JAMES L. RUTLEDGE, Department of Physics OIdahoma State University, StlUwater
More informationDefine the notations you are using properly. Present your arguments in details. Good luck!
Umeå Universitet, Fysik Vitaly Bychkov Prov i fysik, Thermodynamics, 004, kl 9.005.00 jälpmedel: Students may use any book(s) including the textbook Thermal physics. Minor notes in the books are also
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationANALYSIS OF ASPIRIN INFRARED (IR) SPECTROSCOPY AND MELTING POINT DETERMINATION
Chem 306 Section (Circle) M Tu W Th Name Partners Date ANALYSIS OF ASPIRIN INFRARED (IR) SPECTROSCOPY AND MELTING POINT DETERMINATION Materials: prepared acetylsalicylic acid (aspirin), stockroom samples
More informationarxiv:condmat/9711004v1 [condmat.suprcon] 2 Nov 1997
to be published in: J. Phys. Chem. Sol. arxiv:condmat/9711004v1 [condmat.suprcon] 2 Nov 1997 The dimpling in the CuO 2 planes of YBa 2 Cu 3 O x (x=6.8066.984, T=20300 K) measured by yttrium EXAFS
More informationSection 3: Crystal Binding
Physics 97 Interatomic forces Section 3: rystal Binding Solids are stable structures, and therefore there exist interactions holding atoms in a crystal together. For example a crystal of sodium chloride
More informationUnit 12 Practice Test
Name: Class: Date: ID: A Unit 12 Practice Test Multiple Choice Identify the choice that best completes the statement or answers the question. 1) A solid has a very high melting point, great hardness, and
More informationTrading activity as driven Poisson process: comparison with empirical data
Trading activity as driven Poisson process: comparison with empirical data V. Gontis, B. Kaulakys, J. Ruseckas Institute of Theoretical Physics and Astronomy of Vilnius University, A. Goštauto 2, LT008
More informationAppendix I: Cryogenic Reference Tables
Appendix I: Cryogenic Reerence Tables Appendices 217 Appendix I: Cryogenic Reerence Tables Cryogenic heat low calculations The heat low Q conducted across small temperature dierences can be calculated
More information3. Diodes and Diode Circuits. 3. Diodes and Diode Circuits TLT8016 Basic Analog Circuits 2005/2006 1
3. Diodes and Diode Circuits 3. Diodes and Diode Circuits TLT8016 Basic Analog Circuits 2005/2006 1 3.1 Diode Characteristics SmallSignal Diodes Diode: a semiconductor device, which conduct the current
More informationSome Features of the Transport of Charge Carriers in the Grain Boundaries of Polycrystalline Silicon
International Journal of Advanced Research in Physical Science (IJARPS) Volume 1, Issue 6, October 2014, PP 1217 ISSN 23497874 (Print) & ISSN 23497882 (Online) www.arcjournals.org Some Features of the
More information